mechanisms of diffusion in materials - mit .self-diffusion of solute atoms via vacancy mechanism
Post on 11-Jun-2018
Embed Size (px)
3.205 L4 11/7/06
Mechanisms of Diffusion in Materials
A final point on interdiffusion The composition profiles resulting from inter-
diffusion are generally constrained by phase equilibria. Consider the an IrRe diffusion couple annealed at 2400C:
Equilibrium diagram Diffusion couple
23.205 L4 11/7/06
Now consider the OsW system at 2200C :
In this case, a couple initially between pure Os and pure W can form an intermediate phase, , in the interdiffusion zone. If forms, the resulting composition curve will have two discontinuities.
33.205 L4 11/7/06
Illustration of interphase layer growth in XY alloy interdiffusion
Video clip from Diffusion in solid metalmultiphase system, V. Ruth (Universitt Oldenburg), K. Schaar, J. Thienel, and H.G. Graske (Institut fr de Wissenschaftlichen, Gttingen) IWF, Gottingen 1986
43.205 L4 11/7/06
Atomistic mechanisms for diffusion in crystals
Given sufficient thermal energy, an atom can
move from one site to another in a crystal.
Most diffusion in crystals occurs by either the vacancy mechanism or the interstitial mechanism.
53.205 L4 11/7/06
Figures removed due to copyright restrictions.See Figures 8.2 and 8.7 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter.Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891.
Atomistic mechanisms, contd
Additional mechanisms include the interstitialcy mechanism in crystals containing significant numbers of self-interstitials (e.g., produced by irradiation); and the reptation mechanism in molten (hence non-crystalline) polymers.
Interstialcy Reptation 63.205 L4 11/7/06
Atomistic mechanisms, contd Jumps of vacancies and interstitials are thermally
activated, and jumps occur at a jump rate, ,
" # = $ exp %Gm kT( )[ ]
is an attempt frequency typically ~1013 s1; and Gm is the free energy of migration.
The total jump frequency, , is = z , where z is the coordination number (z = 12 in f.c.c.).
73.205 L4 11/7/06
Figure removed due to copyright restrictions.See Figure 7.2 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter.Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891.
Diffusion and random walks
During self-diffusion, vacancies and interstitials execute a random walk among sites in the crystal structure: the trajectories they follow involve a series of discrete jumps, and each jump is uncorrelated with the previous jump.
Illustrate the effects of a vacancy executing a random walk in a diffusion couple via Java applet
83.205 L4 11/7/06
Diffusion & random walks, contd
Mean-square displacement from a random walk of
n jumps each of length r:
R2 = nr2
and for a random-walking vacancy or interstitial, the self-diffusivity in three-dimensional systems is given by:
93.205 L4 11/7/06
Diffusion & random walks, contd
Diffusion in alloys: intrinsic diffusivity and
These can involve correlated jumps and the resulting value of the mean square displacement can be either greater than, or less than, that for self-diffusion. The correlation factor, f, accounts for the extent of correlation, with f = 1 for uncorrelated jumps:
R2 = nr2 " f and D =
103.205 L4 11/7/06
Self-diffusion of interstitials
Involves only random walk of the interstitial species, and thus
DI ="I r
z # " I r2
mkT( )[ ] &1
mk[ ] & exp %HIm kT( )[ ]
Note that interstitial motion is uncorrelated, so f = 1.
113.205 L4 11/7/06
Self-diffusion of vacancies
Involves only random walk of vacancies, and thus
z # " Vr2
mkT( )[ ] &1
mk[ ] & exp %HVm kT( )[ ]
Note that vacancy motion is uncorrelated, so f = 1.
123.205 L4 11/7/06
Self-diffusion of solute atoms via vacancy mechanism
Involves exchange of randomly walking vacancies with the solute atom, A, and thus the atom jump frequency must relate to both the vacancy jump frequency and the probability that a site adjacent to the solute atom is vacant, XV. XV is equal to the equilbrium fraction of vacant sites,
XV = exp "GVf
kT( )[ ] = exp SVf k[ ]exp "HVf kT( )[ ]
133.205 L4 11/7/06
Self-diffusion of solute atoms via vacancy mechanism, contd
Using equations for D and
6exp $ GV
f +GVm( ) kT( )[ ] f
f + SVm( ) k[ ]exp $ HVf +HVm( ) kT( )[ ] f!
"A = XV"V = XV z # " V
The correlation factor, f, for vacancy diffusion in metals is about 0.7 and can be calculated more precisely for various specific cases.
143.205 L4 11/7/06